© Universiti 'Ieknologi Malaysia
Surface Characterization by X-Ray Photoelectron Spectroscopy of Polyethersulfone Hollow Fiber Membranes Modified with Surface
I 12&3" A '12 MRS l' 3 D I' 4& T M 5
N. Bo ong , , .F.Ismail", . . atm", . xana . atsuura
lAdvanced Membrane Research Centre, Faculty Of Chemical& Natural Resources Engineering, Universiti 'Ieknologi Malaysia (UTM), 81310 Skudai, Ichor Malaysia
"Dept, of Environmental Engineering, Faculty of Civil Engineering, Universiti 'Ibknologi Malaysia (UTM), 81310 Skudai,
3Civil Engineering Programme, School of Engineering & IT, Universiti Malaysia Sabah (VMS), 88999 Kota Kinabalu, Sabah, Malaysia
4&5Industrial Membrane Research Laboratory, Dept. of Chemical and Biological Engineering, University of Ottawa, 161 Louis Pasteur St, Ottawa, Ont. ION 6N5, Canada
Novel charged-surface modifying macromolecules (cSMMs) were synthesized and incorporated into polyethersulfone (PES) hollow fiber membranes for water separation application. The macromolecules were synthesized with diisccynate, polypropylene oxide and poly(ethylcne glycol)-hydroxybenzene sulfonate (PEG-HBS). In this study, the surface of polyethersulfone hollow fiber membranes prepared by the phase inversion method was modified using 1 wt.% of SMM and 22 wt.% PES concentration in the polymer casting solution. The effect of cSMM on PES hollow fiber membrane modification was investigated. Elemental analysis shows enrichment of oxygen and sulfone on the modified PES membrane bulk properties. In addition, the glass transition temperature confirms the miscibility of the cSMM in PES. Important relations between surface characteristics due to SMM modification with the PES membrane for water separation performance with respect to XPS characterization also highlighted.
Keywords: Surface modifying macromolecule; polyethersulfone hollow fiber membranes; surface modification, x-ray photoelectron spectroscopy
Nanofiltration technology in water application has been widely studied due to its ability to remove hardness, organics and particulate contaminants and to reduce ionic strength of a solution (Hilal et al.,2004) and to reject organic solutes more effectively than ultrafiltration (Schafer, 2001).
Most of the commercially available nanofiltration membranes are composite polyamide membranes prepared by interfacial polymerization (Kesting,
>I< Corresponding to:N. Bolong (email: email@example.com)
1985). However, the drawbacks of polyamide membranes is their susceptibility to free chlorine and alkaline which causes degradation of the amide group. In this work, nanofiltration is developed by a new approach based on polyethersulfone (PES).
PES is a polymer closely related to polysulfone (PS) and has a high glass transition temperature of 230'C. It has advantages of good membrane forming properties (an important criteria in hollow fiber formation), high mechanical and chemical stability, commercial availability and relatively low cost. PES has the best characteristic of polymers such as segmental flexibilityand processability and capability to be constructed in module forms
(Mahajan, 2000). However, PES polymers being slightly hydrophobic, are not suitable for RO or NF applications without further modifications by suitable chemical reactions like sulfonation (Dey, 2004).
One of the key factors to control membrane properties and structures for achieving the required performance is the alteration of the membrane surface. To modify membrane surface, various methods have been developed such as cross-linking, plasma treatment, grafting technique etc. (Du and Zhou, 2003; Castilhoet al.,2002).
However, it would be desirable to modify the membrane surfacebya simple single-step casting procedure, which is enabled by blending surface modifying macromelocules (SMMs) into the polymeric casting solution, as employed in this work. In this method, only a small quantity of active additive is required (Khayet et al., 2003). The active additive, namely surface modifying macromolecule (SMM), has the ability to migrate preferentially toward a polymer-air interface at membrane surface due to thermodynamic ineompability between the host polymer and SMM (Suketal.,2006). In particular, blending of SMMs that carry a charged functional group (cSMM) can increase the surface charge density of the membrane.
The objective of this work is to evaluate the PES-cSMM miscibility, thus evaluating the feasibility of spinning cSMM blended hollow fibers, to confirm the presence of cSMM in at the surface of the hollow fiber and to study the surface characteristics of the hollow fiber. In order to understand the surface properties towards its separation performance, x-ray photoelectron spectroscopy (XPS) is used to analyze the surface chemical structure olthe hollow fibers.
2.0 EXPERIMENTAL METHODS
2.1 cSMM Synthesis and Hollow Fiber Membrane Fabrication
Material.s used in this study are as follows;
polyethersulfone (PES, Radel A-300, Amoco Chemicals, Germany); N-mcthyl-2-pyrrolidinone (NMP, anhydrous 99.5%), N,N-dimethylacetamide (DMAc, 99+%), N,N-dimethylacetamide (DMAc, 99+%), methylene bis-p-phenyl diisocyanate (MDI), Hydroxybenzenesulfonic acid, sodium salt dehydrate (HBS, 98%), Poly(ethylene glycol)
(PEG, 400 Da) and Diethylene glycol(DEG) all supplied from Sigma-Aldrich, Inc., USA.
The charged-SMM (cSMM) used for dope formulation in this work were laboratory synthesized by the method(Bolong etal., 2009, Mohd Norddinetal., 2008), and have the structures shownin Figure 1.
Based on the soft-segment of the polyurethane prepolymer, namely polyethylene glycol (PEG), and the end capping group, namely hydroxybenzene sulfonate sodium salt (HBS). The utilized cSMM in this work is called poly(ethylene glycol)- hydroxybenzene sulfonate (PEGHBS) according to their soft segment and end-capped.
The cSMM was synthesized using a two-step solution polymerization method. The initial step involved the reaction of methylene bis-p-phenyl diisocynate (MDI) with poly (ethylene glycol) (PEG) in solvent N,N-dimethylacetamide (DMAc). This mixture formed a urethane prepolymer solution. The prepolymer is a blocked- segment of urethane oligomer, poly(4,4'- diphenylenemethylene propyleneurethane) having both ends capped with isocyanate. The second step is the end-capping step by the addition of
O H H O O H H O
•..., _-." - ---.,.,...• ,
Hydroxybenzene '••••••••••••••••••••••••••" ••••••••••••••••---•••' PEG400 ••- -••••••~•••••••••••••••_•••_-... Hydroxybenzene
sulfonate(HBS) Methylenediisocyanale(MDI) Methylenediisocyanate(MOl) sulfonate (HBS)
Figure 1 Chemical structures of poly(ethylene glycol)-4,4' methylene bis(phenyl isocyannate- hydroxybenzene sulfonate
(R+MDI+R) in DMAc (48-50°C) 24 h stirred Thermometer -/
Added drop wise
, - - _~'7
0.03 mol MDlin 50 mL DMAc
r " :----~,
1React for 3 hours , I - - - r - - - I...
~ / '
1- _ .• - -
0.02 mol R in 100 mL DMAc
Added drop wise
. , - - - - ' - - - -...
0.02 mol I-IBS in 50 mL DMAc
Figure 2 Synthesis procedure of charged surface modifying macromolecule (cSMM) Poly(ethylene glycol)A,4' methylene bis(phenyl isocyannate- Hydroxy-benzene sulfonate (PEG-MDI-HBS) in reaction vessel
hydroxybenzene sulfonic acid (HBS). This pre- polymerisation and end-capping process were performed in a controlled atmosphere of purified nitrogen in a reaction vessel. To ensure the elimination of the effects of moisture, all the glasswares were dried at 100De and DMAc was degassed prior to use. The detailed procedure was outlined in Figure 2.
After the resulting solution of cSMM was left under stirring for 24 h at 48-50°C, the cSMM was added dropwise into distilled water under vigorous stirring to precipitate cSMM. The precipitated cSMM was slightly elastic but it was possible to cut it into small pieces. Those pieces were further washed three times and kept immersed in distilled water for 24 hrs under stirring to leach out residual solvent. They were then placed in an aluminum foil and dried in an air circulation oven at50°C for 5 days, by which a constant weight of approximately 10 gwas obtained. The cSMMwas stored in a glass bottle wrapped with aluminum foil, which was then placed in a desiccator.
Hollow fiber membranes were fabricated in the laboratory using a simple phase inversion technique. The hollow fiber membranes were spun at 5ernair gap using water as coagulant both in the coagulation tank and in the bore fluid. Prior to spinning, a spinning dope consisting of PES, water (Deionised), cSMM and N-methyl-2-pyrrolidinone was prepared by the procedure described elsewhere (Bolonget al., 2008) to produce an asymmetric hollow fiber membrane.
2.2 Elemental Analysis and Differential Scanning Calorimetry (DSC)
The bulk elemental composition (carbon, hydrogen and sulfur) for the modified and unmodified hollow fiber membranes was determined by elemental analyzer (Perkin Elmer PE2400 Series II, USA).
The miscibility of PES-cSMM blend was evaluated by measuring the glass transition temperature (Tg) of the polymers using a
Table 1 DSC scan midpoint temperature and bulk atomic percentage of membranes compositions as shown in Table 1. All the fabricated hollow fiber membranes were dissolved using N-methyl-2-pyrrolidinone (NMP) and only SMM 1%weight was needed to cover the membrane surfaces (Ranaet al.,2006) and also to avoid massive changes to the base material.
A well known method of thermal characterization is differential scanning calorimetry (DSC), in which the thermal property is monitored as enthalpy change. A miscible blend exhibits a single Tg whereas an immiscible blend shows multiple Tgs (Kapantaidakiset al., 1996).
The midpoint Tg, given as the temperature at which half of the total change in the specific heat capacity occurs, is summarized in Table 1.
All membranes exhibited a single Tg, which implies the homogenous blend of cSMM (PEGHBS) with PES. The Tg's of all the hollow fibers of multi-components are less than the hollow fiber 01 the single pure PES component.Itseems that the addition of cSMM reduces Tg considerably but for the formulation that includes water, Tg partially comes back to the nearly original value of pure PES. Compositional variation ofTg is mainly governed both by the interaction between the components and the change in chain flexibility with the compositional change (Kim and Jang, 2002) .
The bulk elemental analysis of the fabricated hollow fibers shows only a slight change in Tg when cSMM is added (Table 1). The blends of PEGHBS show an increase of in sulfur content with occurrence of nitrogen which is attributed to the amide group in the PEGHBS.
Bulk Elemental (Atomic ratio) differential scanning calorimeter (Mettler Toledo
DSC 822e). Samples were cut into small pieces, weighed to 6±0.5 mg and placed in a pre-weighed aluminum crucible. Then, the sample was heated from 25 to 250"C with a heating rate of 20"C min-I Tg of the sample was determined as the midpoint temperature of the transition region in the heating cycle.
2.3 X-ray Photoelectron Spectroscopy (XPS)
X-ray photoelectron spectroscopy (XPS) or also known as electron spectroscopy for chemical analysis (ESCA) is particularly well suited for examining the skin layer of a membrane, sinceit probes only at resolution depth of -10 nm into the membrane surface. XPS analyses were carried out with Axis-165 ultra (KratosAnalytical, Shimadzu, Japan) using MgKa exciting radiation (hv=1 253.6 eV). The excitation source was run at 15 kV and 10 rnA.To compensate for surface charging effects, all binding energies were referenced to the CIs neutral carbon peak at 284.5 eV
Surface elemental stoichiometries were determined from the sensitivity-factor-corrected peak area ratios, and the software XPSpeak 4.1 was used to fit the XPS spectral peaks. Prior to XPS tests, hollow fiber membranes were rinsed in distilled water and then dried in an vacuum oven at a temperature of 30°C for 8 hours to remove moisture or water, which would affect the XPS sampling environmentduring chamberevacuation, and consequently ensure sufficient vacuum on the measurement system. Hollow fiber membrane sample was compactly arranged and directly pressed to a self-supported (10 xl0 nun) disk and mounted on a sample holder before being transferred into the analyzer chamber.
3.0 RESULTS AND DISCUSSION
Membrane Tg CC) composition
C H N S 0
3.1 SMM and Fabricated Hollow Fiber PES (22) 231 3.29 7.32 0.00 0.152.97
Membranes Properties PES-PEGHBS
(22/1) 208 3.89 6.53 0.08 0.222.41 The hollow fibers were spun by the dry-wet phase PES-PEGHBS-
inversion technique using dopes of three different Water(22/1/5) 228 3.50 6.94 0.Q7 0.192.75
3.2 X-ray Photoelectron Spectroscopy (XPS) Analysis
The surface compositions of the modified and unmodified hollow fiber membranes were determined using XPS. X-ray resolution data was collected at incident x-ray angle (8) of 90°, The 8 angle is measured relative to the horizontal plane of the sample surface.Itrepresent the top <10 nm of the membrane surface. The survey of the XPS spectrum confinued the presence of the desired elements in the hollow fiber samples as shown in Figure 3. Wide scan of samples displayed the peal"
arising from ionization of core electron of C, N,
and S. Weak peak appearing at 402 eV for modified PES notation for N1s observed due to amide N-R of PEGRBS, indicating surface modification but the peak is too small for further analyses and may not be the main concern of the modification study. On the other hand, CIs, 01s, S2p and S2s peal, appeared at 280-290 ev, 530- 540 ev, 170-180 and 240-250 ev respectively.
To further investigate the effect of PEGRBS blending, further analysis was conducted on the states of C and 0 atoms. The analysis was limited to the PES (without blending) and PES-PEGRBS- Water membranes. This is because the PES- PEGRBS-Water was found to exhibit belter performance than the PES-PEGRBS membrane.
For example, pure water permeation was 11.1 L/m2h.Bar and 4.5 L/m2h.Bar,respectively, for PES-PEGRBS-Water and PES-PEGRBS membrane (Bolonget al.,2009).
In order to reveal the states of the atoms of the modified (PES-PEGRBS-Water) and the unmodified (PES) membrane, the high resolution XPS spectra of CIs and 01s were analyzed by peal, fitting based on Gaussian functions. In Figure 4 and 5 respectively, the XPS spectra of the CIs and 01s region are shown in high resolution for both the modified PES-PEGRBS-Water and unmodified PES membranes.
Figure 4 shows the CIs spectra.Itis difficult to make complete analysis of the CIs spectra due to
1800 1600 1400 1200 1000 800 600 400 200
o1000 800 600 400 200
(b) and (c) are Polyethersulfone blended with PEGHBS (Figure 1)
Binding energy (eV)
Figure 3 XPS Wide scan (0-1100 eV) of hollow fiber samples (a) PES unmodified, (b)PES/PEGRBS and (c)PES/Water/PEGRBS
many different chemical states of carbon atoms.
Hence, the CIs spectrum were deconvoluted into 3 main peaks for unmodified PES whereas 4 main peaks for modified PES, This is because the observed spectrum for modified PES has broader left shoulder compared to unmodified PES indicating of surface modification due to PEGHBS blends. The main peak at the binding energy of 284.4 ev can be assigned to the phenyl carbon (Folkessonet al., 1998) that exists in the backbone of both membranes. Itis reasonable to note that CIs spectra shows a broad line width structures, since it contains contributions of several carbons in different chemical sites. Yet, the correspond binding energy reported by other study (Wavhal et al., 2002) reveals similar spectra for the unmodified PES membrane studied in this work.
As shown in Figure 4, both PES membranes confirm the occurrence of C-S and c-o at respective binding energy of 285.3 eV and 286.2 eV The carbon atom bonded to the sulfur atom C- S is present in both types of membranes, however due to modification of PEGHBS, stronger peak
(a) PES without PEGHBS
Binding Energy leV)
was observed, and that caused a significant revolution at left shoulder of CIs spectrum.
Another prominent peak at 288eV that attributed to C= 0 configuration (Ratset al., 1995) reveals presence of PEGHBS via the MDI components,inthe modified PES-PEGHBS-Water membrane.
The 01 s spectrum of the membranes was deconvoluted by peak fittings as depictedinFigure 5 (a) and (b). Since both membranes base polymer is PES, the peak at 530.7 eV that assigned for the oxygen present in the sulfonic acid group (C-S=O) (Nasef et al., 2002) and at binding energy of 531.7 eV that is contributed from O=S=O (Wavhal et al., 2002)was depicted. By comparison of the 01s spectrum of modified PES membrane with that of original or unmodified membrane, it is found that the C-O·C peak (532.9 eV) has impose left shoulder severely compared to modified PES.
The reason might due to the overlapping peak of c=o (at 531.5eV) with 0=5=0 implicate the migration of oxygen atom at membrane surface due to cSMM (i.e PEGHBs) added.
(b) PES with PEGHBS
Binding Energy (eV)
Figure 4 The XPS spectrum of CIs region for the (a) PES unmodified and (b) PES modified with PEGHBS
(a) PES without PEGHBS
5 1 Binding Energy (eV)
(b) PES with PEGHBS O=S=O/C=O
Binding Energy (eV)
Figure 5 The XPS spectrum of 01s region for the (a) PES unmodified and (b) PES modified with PEGRBS
The following conclusions can be drawn from the experimental results.
(1) Elemental analysis showed the increase in N and S content in the cSMM (PEGHBS) blended membranes. This is an evidence for the presence of PEGHBS in the membranes surface and hence confirms the move-up towards membrane surface.
(2) According to DSC analysis, only a singleTgs were obtained for the cSMM blended membranes, this is the verification for the perfect miscibility of PEGHBS in PES.
(3) The left shoulder of the main CIs peak was enhanced by the peak corresponding to atom carbon binding with sulfur. The right shoulder of the main 01 s peak was enhanced by the peak corresponding to sulfonic acid (S=O). All of the XPS data analysis suggests the modification of PEGHBS at PES membrane surface, which successfully migrated at membrane surface and indeed present in the modified PES-PEGRBS- Water membrane.
This research has been financially supported by Ministry of Higher Education, Malaysia (MOHE) and UniversitiMalaysia Sabah (UMS).The author wishes to thank Prof. Zeng Hua Chun from the Department of Chemical and Biomolecular Engineering, National University of Singapore (NUS), Singapore; who gave us the possibility to undertake visiting scholar progamme at NUS and access to the elemental analysis andXPS facility.
 Abdureyim, A., K. K. Okudaira, Y Harada, S. Masuda, M. Aoki,K.Seki, Eisuke Ito and N. Ueno, 2001. Characterization of 4- Mercatohydrocynnamic Acid Self- assembled Film on Au(111) by means of X-ray Photoelectron Spectroscopy.
[. of Electron Spectroscopy and Related Phenomena. 114-116:371-374.
 Bolong, N., A.F.Ismail, M.R.Salim, D. Rana and T Matsuura. 2009. Development and
Characterization of Novel Charged Surface Modification Macromolecule to Polyether- sulfone Hollow Fiber Membrane with Folyvinylpyrrolidone and Water.
 Bolong, N.,A.E Ismail,M. R Salim, D. Rana andT.Matsuura. 2008. Inflnence of Surface Modifying Macromolecules (SMMs) on Polyetbersulfone Hollow Fiber Membranes for Water Separations. Presented on 6th Regional Symposium on Membrane Sci.&
Tech. 2008, 13-15 August Phuket Thailand.
 Castilho,L. R, W D. Deckwer and E B.
Anspach. 2002. Influence of Matrix Activation and Polymer Coating on the Purification of Human IgG with Protein A Aflinity Membranes.f.Membr. Sci.172:269.
 Dey, T. K, R C. Bindal, M. S. Hamra and B.
M. Misra. 2004. Dependence of Performance of Poly(Sulfone Co-Amide) Membranes on Compositional Variation of Casting Solntion and Coagnlation Media - Development of Reverse Osmosis and Nanofiltration Membranes. Separation Science& Technology.39: 581-601.
 Dn, R andJ. Zhao. 2003. Positively Charged Composite Nanofiltration Membrane Prepared by Poly(N,N-dimethylaminoethyl methacrylate)/polysulfone.
 Folkesson, B.,P.Sundberg and R Larsson.
1988. On the Core Electron Binding Energy of Carbon and the Effective Charge of the Carbon Atom. Journal of Electron Spectroscopy and Related Phenomena. 46:
 Franks, E, 1988.Water Science Reviews 3:
Water Dynamics. Cambridge University Press. UK
 Hilal N., H. AI-Zoubi, N.A.Darwish,A.W Mohammad and M. Abu Arabi, 2004. A Comprehensive Review of Nanofiltration Membranes: Treatment, Pretreatment, Modeling and Atomic Force Microscopy.
Desalination. 170: 281.
 Hollinger, G., G. Marest, H. [affrezic, J.
Tonsset and N. Moncoffre. 1985.
Temperature Influence during Nitrogen Implantationinto Steel.NuclearInstruments
and Methods in Physics Research B7/8.177-183.
[11J Kapantaidakis, G. C., S.P. Kaldis, X. S.
Dabou and G.P.Sakellaropoulos. 1996. Gas Permeation through PSF-PI Miscible Blend Membranes.
f.Membr. Sci.110: 239.
 Kesting, RE. 1985. Synthetic Polymeric Membranes.New York: Wiley.
 Khayet, M., D. E. Suk, R M. Narbaitz, J.P.
Santerre andT.Matsuura. 2003. Study on Surface Modification by Surface-modifying Macromolecules and its Applications in Membrane-separation Processes.
Polym. Sci.89: 2902-2916.
 Kim, J. H. and ]. [ang. 2002. Thickness and Composition Dependence of the Glass Transition Temperature in Thin Homogeneous Polymer Blend Films.
Macromolecules. 35: 311.
 Mahajan, R. 2000. Formation, Characterization and Modeling of Mixed Matrix Membrane Materials, Ph.D.
Dissertation, The University of Texas at Austin.
 Mohd Norddin, M. N. A., A. E Ismail, D.
Rana,T. Matsuura and S. Thbe. 2008. The Effect of Blending Sulfonated Poly(ether ether ketone) with VariousCharged Surface Modifying Macromolecules on Proton Exchange Membrane Performance.
Membr. Sci.In Press. doi:1O.1016/j.memsci.
[17J Monlder,J. E, W F Sticlde,P.E. Sobol and K D. Bomben. 1995. Handbook of X Ray Photoelectron Spectroscopy: A Reference Book of Standard Spectra for Identification and Interpretation of Xps Data. Physical Electronic Publishers. Perkin Elmer Corp.
 Mustin, C. Ph. De Donato, R Benoit and R Erre. 1993. Spatial Distribution of Iron and Sulphure Species on the Surface of Pyrite.Applied Surface Science. 68: 147- 158.
 Nasef, M. M. and H. Saidi. 2002. Post- mortem Analysis of Radiation Grafted Fuel Cell Membrane using X-ray Photoelectron Spectroscopy.
f. ofNew Mat.
Electrochemical Sys. 5: 183-189.
 Poleunis, C. L., T. Weng, M. Sclavons, P.
Bertrand, P. Franquinet, R Legras and V Carlier. 1995. Sizing Removal and Functionalization of Carbon Fiber Surface Studied by Combined TOF SIMS and XPS.
Journal Adhesion Sci. Technol. 9. 7: 859- 871.
 Rana, D., T. Matsuura, R M. Narbaitz and C. Feng. 2005. Development and Characterization of Novel Hydrophilic Surface Modifying Macromolecule for Polymeric Membranes.
f.Membr. Sci. 249:
 Rats, J. D., L. Sevely, RVandenbulcke, R Benoit, R Erre, V Herbin and V Serino 1995.
Characterization of Diamond Films Deposited on Titanium and its Alloys. Thin Solid Films. 270: 177-183.
 Schafer, A. I. 2001. Natural Organics Removal Using Membranes: Principles, Performance and Cost.TechnomicPulishing co. Inc, USA
[24J Suk, D. E., T. Matsuura, H. B. Park andY. M.
Lee. 2006. Synthesis of a New Type of Surface Modifying Macromolecules (nSMM) and Characterization and Testing of nSMM Blended Membranes for Membrane Distillation.f. Membr. Sci. 277: 177.
 Thompson,A.C and D. Vaughn.2001. X-ray Data Booklet, US Dept. of Energy (DE- AC03-765F00098).
 Wagner, C. D., W M. Riggs, L.E.Davis, J.F.
Moulder and G. E. Mullenberg. 1979.
Handbook of X-ray Photoelectron Spectroscopy. Perkin-Elmer Corp., Eden Prairie, MN, USA.
 Watts, J. F and J. Wolstenholme. 2003. An Introduction to Surjace Analysis by XPS and AES.John Wiley& Sons, USA.
 Wavhal, D. Sand E. R Fisher. 2002.
Hydrophilic Modification of Polyether- sulfone Membranes by Low Temperature Plasma-induced Graft Polymerization.